polymers are technologically very important. A good example is polystyrene (PS). If a special catalyst is used in its synthesis it is possible to obtain the syndiotactic version of this polymer, but most industrial polystyrene produced is atactic. The two materials have very different properties because the irregular structure of the atactic version makes it impossible for the polymer chains to stack in a regular fashion. The result is that, whereas syndiotactic PS is a semicrystalline material, the more common atactic version cannot crystallize and forms a glass instead. This example is quite general in that many polymers of economic importance are atactic glass formers. Eutactic polymers In eutactic macromolecules, substituents may occupy any specific (but potentially complex) sequence of positions along the chain. Isotactic and syndiotactic polymers are instances of the more general class of eutactic polymers, which also includes heterogeneous macromolecules in which the sequence consists of substituents of different kinds (for example, the side-chains in proteins and the bases in nucleic acids). Head/tail configuration In vinyl polymers the complete configuration can be further described by defining polymer head/tail configuration. In a regular macromolecule all monomer units are normally linked in a head to tail configuration so that all β-substituents are separated by three carbon atoms. In head to head configuration this separation is only by 2 carbon atoms and the separation with tail to tail configuration is by 4 atoms. Head/tail configurations are not part of polymer tacticity but should be taken into account when considering polymer defects. Techniques for measuring tacticity Tacticity may be measured directly using proton or carbon-13 NMR. This technique enables quantification of the tacticity distribution by comparison of peak areas or integral ranges corresponding to known diads (r, m), triads (mm, rm+mr, rr) and/or higher order n-ads, depending on spectral resolution. In cases of limited resolution, stochastic methods such as Bernoullian or Markovian analysis may also be used to fit the distribution and predict higher n-ads and calculate the isotacticity of the polymer to the desired level. Other techniques sensitive to tacticity include x-ray powder diffraction, secondary ion mass spectrometry (SIMS), vibrational spectroscopy (FTIR) and especially two-dimensional techniques. Tacticity may also be inferred by measuring another physical property, such as melting temperature, when the relationship between tacticity and that property is well-established. References External links Tacticity @ École Polytechnique Fédérale de Lausanne Application of spectroscopy in polymer charactisation @ University of California,